APLICACION DE NANOTUBOS MULTICAPA EN LA RESISTENCIA MECANICA DE NUEVE MADERAS COMERCIALES DE COSTA RICA.
APLICACAO DE NANOTUBOS MULTICAMADA EM RESISTENCIA MECANICA DE NOVE MADEIRAS COMERCIAIS DA COSTA RICA
Carbon nanotubes (CNTs) are carbon allotropes such as diamond, graphite or fullerenes, and its structure can be like a graphene sheet rolled on itself (Lariza et al., 2012). They are cylinders of one or more layers with open or closed ends (De Volder et al., 2013), can have a diameter of nanometers and their length can reach up to 1mm, so the ratio of length-width is very high (Perez, 2010). The commercial interest in CNTs is reflected in its production capacity, which exceeds several thousand tons per year.
The characteristic advantages of CNTs like high mechanical strength and good thermal stability (Orinakova and Orinak, 2011) make them important for a perfect scientific environment product (Perez, 2010). However, the disadvantages involve adoption of regular shapes like pentagons and heptagons during mass production, which is not the perfect union of the CNT and hence the properties can be degraded (De Volder et al., 2013). Moreover, lack of solubility in organic solvents or aqueous solutions is also a drawback of these structures (De Volder et al., 2013), but they can undergo chemical reactions that make them soluble in various solvents, and can be integrated with inorganic, organic and biological systems (Saeb et al., 2015), a process known as 'functionalization' of the nanotubes.
CNTs have several applications and can be utilized at different sectors. In medicine, they can be used for diagnosis and treatment of cancer, nervous system disorders and infectious diseases (Zhang et al., 2010). They can be exploited in compound materials as electrical conductive fillers in plastics; to improve fiber compounds among wind turbine blades or vanes boats; in paints to help reducing biofouling of ship hulls (De Volder et al., 2013); and very importantly as an anticorrosive coating for metals to improve the rigidity of coating (De Volder et al., 2013).
On the other hand, the complex structure of the wood cell and the physical and mechanical properties of its wall has attracted the attention of scientists, and has recently led to the study of the effects of nanotechnology on wood structure (Moon et al.; 2006; Kamel, 2009). Among many studies, the major concern has been evaluating the possibility of working with wood in a nano scale to have more absorbent, lightweight and strong products (Shmulsky and Jones, 2011). For example, Kordkheili et al. (2012) have studied the influence of mixture of cement, wood fiber and CNT's, and they found that the static bending was higher when a mixture of 1.5% multilayer nanotubes (MWCNT), 20% fiber and 43% of cement is used. Another study, in Ficus hispida, has shown the improvement in structural properties (Hazarika and Maji, 2014). This type of wood grows in the tropics, it is soft and is not suitable for structural applications due to their poor physical and mechanical properties. However, hydroxyl group multilayered nanotubes (MWCNT-OH) in different concentrations were added to wood in a solution of ethanol and potassium hydroxide mixed with a copolymer of melamine and formaldehyde (MFFA) in order to determine their influence on the wood structure. The hardness properties, bending and tension of the wood were found highest when the concentration of the MWCNT-OH was 1.5, which coincides with the study conducted by Fu et al. (2010).
They also found that the thermal stability and flammability properties of polypropylene (PP)/wood flour enhances these properties when CNTs were added.
In Costa Rica, 17.5% of wood is used in the manufacture of furniture and an important part of the latter is exported (ONF, 2013). It is estimated that about 15 different wood species are used for manufacturing of furniture and these woods comes from plantation or natural and secondary forests stands (ONF, 2013). However, these species are of medium density and in some cases have limited resistance (Serrano and Moya, 2011), so better strength and performance with MWCNT may be an option and can add value to these woods.
The aim of this work was to study the mechanical properties (static bending, tension parallel to the fiber, lateral and axial hardness, compression perpendicular to grain, shear parallel to grain) of nine tropical species by introducing a solution of multilayer carbon nanotubes functionalized with hydroxyl groups (MWCNT-OH) at two concentrations (0.05 and 0.10%).
Materials and Methods
Multilayer carbon nanotubes functionalized with hydroxyl groups (MWCNT's-OH) were supplied by CheapTubes Inc. (Cambridgeport, MA, USA). The manufacturer's technical information for nanotubes is: outer diameter of about 50nm, length of 10 to 20[micro]m, purity of 95% and an OH group concentration of 0.5-1.0% by weight.
Nine wood species used in this study were grown in tropical area of Costa Rica. They are cataloged in three groups; i) the species most used in reforestation programs: Gmelina arborea, Tectona grandis (teak) and Acacia mangium, usually employed in lightweight construction; ii) species used in furniture manufacturing: Cordia alliodora, Cedrela odorata and Enterolobium cyclocarpum; iii) species providing potential wood for furniture and construction and in high abundance in the secondary forest: Vochysia ferruginea, Ochroma pyramidale and Goethalsia meiantha. These woods were obtained from sawmills and timber shops near the facilities of the Technological Institute of Costa Rica.
Wood boards used presented a thickness of 6cm and in most cases the width was corresponding to the diameter of the log, which is commonly used as sawing pattern for furniture manufacturing (Serrano and Moya, 2011). The boards were air dried and 45 samples were prepared for each type of mechanical test, according to the ASTM D-143 (ASTM, 2014) standard: compression perpendicular to grain: 2.5x2.5x10.0cm; static bending: 2.5x2.5x41cm; shear parallel to grain: 5.0x5.0x 6.3cm; lateral and axial hardness: 5x5x15.0cm; and tension parallel to grain: test pieces 2.5x2.5x46.0cm.
Characterization of multilayer carbon nanotubes functionalized
The detail of the features, dimensions and other aspects of MWCNT-OH is widely explained by Moya et al. (2015a) and can be summarized as: the MWCNT-OH have the 3-band characteristics of multilayer nanotubes, called D, G, G' (Figure 1), and it differs from non-functionalized nanotubes in the band D. This difference is attributed to defects in the walls of the nanotubes or atoms that have been added to the st ructure of the nanotubes, and the differences in the bands G and G' are produced by st retching in the plane of carbon-carbon bonds in the leaves of graphene, and it also indicates disorders and defects in carbon nanotubes. Concerning the thermal stability, the MWCNT-OH used have the maximum decomposition at ~600[degrees]C, showing that they have better thermal stability than the non-functionalized nanotubes (Figure 1b).
Preparation of the MWCNT-OH solution
MWCNT-OH solutions were prepared by adding 0.03g and 0.015g of MWCNT-OH in 200ml of water for 0.10% and 0.05% concentration, respectively. The prepared MWCNT-OH solutions were sonicated for 5min with an Ultrasonic Processor Model CV18 at an amplitude of 75% at intervals of 45sec, with 10 sec breaks. Then, 200ml of the solution was poured into 3L of water and re-zoned for 25min. The process continued until 15L of solution is left and finally, water was added to have 30 L of total solution.
Impregnation of wood with MWCNT-OH
Samples were placed in an experimental pressure tank commonly used for wood preservation. The process of impregnation of MWCNT-OH solution consist of 30min at -78kPa vacuum, 2h at 690kPa pressure and 15min at -78kPa vacuum. Then, the wet samples were placed in a controlled environment for six months to reach an equilibrium moisture content of 12% (air dried wood).
Absorption and retention-OH MWCNT in wood samples
Wood samples were weighed before and after the impregnation process and two parameters were generated: absorption capacity and retention of MWC NT-OH. The absorption capacity for each sample was calculated as the absorption of the solution in liters per timber volume (Eq. 1), while retaining MWCNT-OH absorption was determined considering MWC NT-OH by wood weight, according to Eq. 2.
Absorption ([L.sub.solucion]/[m.sup.3]) = [(Weight of solution impregned)(kg)*[density.sub.solution] (kg/[m.sup.3])]/[Volume of sample ([m.sup.3])] * [L.sub.solucion]/[m.sup.3] (1)
Retencion = [Absorption([L.sub.solucion]/[m.sup.3])]/ [Volume of sample ([m.sup.3])] * Concentration of nanotubes (mg/[L.sub.solucion]) (2)
Mechanical strength tests
The effect of MWCNT-OH in improving resistance of wood was evaluated by five mechanical tests: static bending, tension parallel to the fiber, lateral and axial hardness, compression perpendicular to grain and shear parallelto grain. These mechanical tests were conducted according to ASTM D-143 standard (ASTM, 2014). For each type of mechanical test, total of 45 samples were used, 15 for each type of MWCNT-OH concentration. The bending, tension parallel to the fiber and hardness tests were performed in a universal testing machine (Tinius Olsen model H10KT) while the cutting tests and compression were carried out in a universal testing machine (Tinius Olsen model LT60).
A descriptive analysis of the parameters studied (with each trial) was performed (mean and standard deviation). Additionally, it verifies whether the variables satisfy the assumptions of normal distribution, homogeneity of variances and the presence of extreme data. Subsequently, an analysis of variance (ANOVA) was applied to verify the effect of the concentration of MWCNT-OH on the mechanical properties studied. Then, the statistical differences between the average were established by a Tukey test at a confidence level of 95%. For that, Statistical Analysis Software (SAS) was used and a comparison was made between the means, whereas figures and tables were made in Excel 2013.
MWCNT-OH absorption and retention
C. alliodora, G. meiantha and O. pyramidale woods showed greater absorption and retention of MWCNT-OH (Table I). O. Pyramidale retained the most MWCNT-OH among the nine species in the treatment of 0.10% whereas T. grandis showed lowest uptake and retention in both MWCNT-OH concentrations.
For this test, O. pyramidale, Vochysia ferruginea, E. cyclocarpum, C. alliodora, G. arborea and T. grandis showed no significant difference in any of the MWCNT-OH concentrations (Figure 2), while A. magnium, C. odorata and G. meiantha exhibited statistical differences. In A. mangium wood, the modulus of elasticity (MOE) of the wood treated with MWCNT's-OH 0.05% has lower compared to control, whereas with the 0.10% treatment no significant difference was found when compared with untreated wood. The same applies to the modulus of rupture (MOR) of wood treated with 0.05% MWCNT-OH; the MOR was statistically lower than the wood without nanotubes. In C. odorata, differences were found when nanotubes were present in the wood. Statistically, MOR of the timber with 0.05% MWCNT-OH was greater than the wood with 0.10% of nanotubes. However, there was no MOR alteration noticed with either of concentration of nanotubes, compared to untreated wood.
In G. meiantha, MOR value was statistically higher in wood treated with 0.10% MWCNT-OH; however, the wood treated with 0.05% MWCNT-OH showed no difference in comparison with untreated wood.
Tension parallel to the fiber
The ANOVA indicated that the species A. magnium, C. alliodora, E. cyclocarpum, G. arborea, O. pyramidale and V. ferruginea showed no significant differences when applied to the different concentrations, while the rest of the species differed (Table II). In C. odorata both treatments had higher values than the control. The treatment of 0.05% had a statistically higher value than the control in the case of G. meiantha, while the 0.10% treatment did not show differences with the control. Similarly, in T. grandis, the 0.05% treatment showed a significant higher value compared to the other treatment and control.
Lateral and axial hardness
In this mechanical test, A. magnium, V. ferruginea, G. meiantha, G. arborea and C. alliodora showed significant differences in at least one of the concentrations of MWCNT-OH (Figure 3). A. magnium presented greater lateral hardness in the concentration of 0.05%, while 0.10% did not show a difference with the wood without MWCNT-OH. Whereas Vochysia ferruginea presented difference in axial hardness. Wood treated with 0.10% MWCNT-OH had less lateral stiffness than the one treated with 0.05% concentration MWCNT-OH. However, G. meiantha presented significantly higher values with the 0.10% concentration of MW CNT-OH and C. alliodora had differences in both lateral and axial hardness in both cases; the treatment of 0.05% had a statistically higher value than the untreated wood. While Gmelina arborea also differ in lateral and axial hardness, in this case the differences are in the treatment of 0.10%, which was statistically greater than wood without MWCNT-OH (Figure 3).
Compression perpendicular to grain
In the compression test, G. arborea, G. meiantha, and O. pyramidale were the only species with significant differences between treatments (Table 3). Gmelina arborea presented a statistically higher value when wood was treated with MWCNT-OH at a concentration of 0.05%, and O. pyramidale and G. meiantha were statistically observed with lower value in treated wood (MWCNT-OH concentration of 0.05%).
Shear parallel to grain
In this strength test, A. magnium and C. alliodora showed some significant differences (Figure 4). In both the species, when wood is treated with MWCNT-OH to a concentration of 0.05%, a significant increase in strength was observed relative to the wood with 0.10% treatment and without MWCNT-OH (Figure 4).
Absorption and retention The behavior of increase in absorption (Table I) with the decrease in wood density is consistent with results of other studies where some form of nanoparticles were used in wood (Moya et al., 2014, 2017). Consistent with the above, it was also found that a greater amount of MWCNT/[m.sup.3] was absorbed in lower density wood, such as O. pyramidale, C. alliodora and G. meiantha, while species like T. grandis and A. mangium, with higher density, the absorption was lower and retained less of MWCNT (Table I).
V. ferruginea had the highest absorption value, unlike O. pyramidale, of low density, which did not present the same absorption as the previous species. The low retention of MWCNT in T. grandis or A. mangium wood is explained by the fact that this wood has a high percentage of heartwood, which is not possible to preserve. Moya et al. (2017) reported that in the vacuum-pressure treatment, penetration is null when there is heartwood; but there is adequate sapwood penetration in these wooden species.
Although several authors had shown that the use of MWCNT-OH improves wood properties (Hazarika and Maji, 2014; Kordkheili et al., 2012), the results of this study were not consistent with them, as most species included show no significant improvement in the mechanical tests performed. This behavior can be attributed to the MWCNT-OH having imperfections or impurities, which do not allow a suitable combination with wood substrates (De Volder, 2013), so this situation cannot allow adequate support of MWCNT-OH and wood.
Another aspect that may be contributing to the ineffectiveness of the strengthening of tropical wood with the injection of MWCNT-OH is the type of functionalization used. The hydroxyl group used in this work to functionalize MWCNT is commonly used as a precursor (Xie et al., 2010) that increases the strength of wood by adding another functional group compatible to wood components.
Although the carboxyl functional group allows interaction with the four hydroxyl groups of the cell wall polymers in the wood fiber, this is used as a crosslinking agent to modify the wood fibers (Xie et al., 2010). The results in the different woods resistance were not as effective. Also, influencing the ineffectiveness of the MWCNT-OH is the variability and complexity of the chemical composition of these tropical species, which also varies between and within species (Kilic and Niemz, 2012; Moya et al., 2015b), so that the functional group of nanotubes might not have a proper interaction with the timber.
Finally, the irregularity presented in the mechanical testing in two concentrations of MWCNT-OH is also an important parameter to demonstrate. For example, G. arborea wood exhibited a greater resistance at 0.05% concentration in comparison to 0.10% in some experiments, but the hardness of the same species showed the opposite effect, the stress value in the 0.05% treatment being higher than 0.10%. This irregularity can be attributed to variability in the wood used. Those samples were extracted from different timber shops, and these are usually not separated according to the different parts of the tree. The fast-growing plantations of wood in tropical regions generally have greater variation in wood properties (Moya and Munoz, 2010).
The vacuum-pressure method can be used for MWCNT injection into wood; however, the hydroxyl group functionalization of the nanotubes is not suitable for a reinforcement of the mechanical properties of the nine commercial species of Costa Rica studied. Furthermore, the strength values of these nine species were not homogenous and it was not possible to establish an effect of MWCNT. With the objective of knowing the effects of MWCNT on wood, it is necessary to standardize some aspects, such as wood precedence. It is also most important to use a type of functionalization that allows greater interaction of MWCNT with wood structure.
The authors thank the Vicerrectoria de Investigacion y Extension, Instituto Tecnologico de Costa Rica (ITCR) for financial support.
ASTM (2014) Standard test methods for small clear specimens of timber ASTM D143-14. Annual Book of ASTM Standards. Vol. 11.06. Philadelphia, PA, USA.
De Volder M, Tawfick S, Baughman R, Hart J (2013) Carbon nanotubes: present and future commercial applications. Sci. 339(6119): 535-539.
Fu S, Song P, Yang H, Jin Y, Lu F, Ye J, Wu Q (2010) Effects of carbon nanotubes and its functionalization on the thermal and flammability properties of polypropylene/wood flour. J. Mat. Sc. 45: 3520-3528.
Kamel S (2009) Nanotechnology and its applications in lignocellulosic composites, a mini review. eXPRESS Polymer Lett. 1: 546-575.
Kordkheili HY, Hiziroglu S, Farsi M (2012) Some of the physical and mechanical properties of cement composites manufactured from carbon nanotubes and bagasse fiber. Mat. Design 33: 395-398.
Kilic A, Niemz P (2012) Extractives in some tropical woods. Eur. J. Wood Prod. 70: 79-83.
Hazarika A, Maji TK (2014) Strain sensing behavior and dynamic mechanical properties of carbon nanotubes/nanoclay reinforced wood polymer nanocomposite. Chem. Eng. J. 247: 33-41.
Lariza M, Lopez I, Saenz A (2012) Nanotubos de carbono: funcionalizacion y aplicaciones biologicas. Rev. Mex. Cs. Farmaceut. 43(3): 9-18.
Moya R, Munoz F (2010) Physical and mechanical properties of eight species from fast-growth plantaion in Costa Rica. J. Trop. For. Sci. 22: 317-328.
Moya R, Ber rocal A, Rodriguez-Zuniga A, Vega-Baudrit J, Chaves-Noguera S (2014) Effect of silver nanoparticles on white-rot wood decay and some physical properties of three tropical wood species. Wood Fiber Sci. 46: 527-538.
Moya R, Rodriguez-Zuniga A, Berrocal A, Vega-Baudrit J (2015a) Effects of adding multiwall carbon-nanotubes (MWCNT) on performance of polyvinyl acetate (PVAc) and urea-formaldehyde (UF) adhesives in tropical timber species. J. Nanomat. 2015: Article ID 895650.
Moya R, Salas C, Ber rocal A, Valverde JC (2015b) Evaluation of chemical compositions, airdry, preservation and workability of eight fast-growing plantation species in Costa Rica. Maderas Bosques 21(Esp.): 31-47.
Moya R, Rodriguez-Zuniga A, Berrocal A, Vega-Baudrit J (2017) Effect of silver nanoparticles synthetized with NPsAg-ethylene glycol (C2H6O2) on brown decay and white decay fungi of nine tropical woods. J. Nanosci. Nanotech. 17: 5233-5240.
Moon RJ, Charles R, Frihart CR, Wegner T (2006) Nanotechnology applications in the forest products industry. For. Prod. J. 56(5): 4-10.
ONF (2013). Usos y aportes de la madera. Oficina Nacional Forestal. San Jose, Costa Rica.
Costa Rica. www.onfcr.org/media/uploads/documents/uyam_ onf_2014_3_af_ultimo.pdf Perez A (2010) Nanotubos de carbono. Rev. Inf. Tecnol. Soc. 10: 1-10.
Orinakova R, Orinak A (2011) Recent applications of carbon nanotubes in hydrogen product ion and storage. Fuel 90: 3123-3140.
Saeb MR, Najafi F, Bakhshandeh E, Khonakdar HA, Mostafaiyan M, Simon F, Mader E (2015) Highly curable epoxy/MWCNTs nanocomposites: An effective approach to functionalization of carbon nanotubes. Chem. Eng. J. 259: 117-125.
Ser rano R, Moya R (2011) Procesamiento, uso y mercado de la madera en Costa Rica: Aspectos historicos y analisis critico. Rev. For. Mesoamer. 9(21): 1-12.
Shmulsky R, Jones D (2011) Forest Products and Wood Science. 6th ed. Wiley. New York, USA. 532 pp.
Xie Y, Zefang X, Timo G, Militz H, Hill C, Steuernagel L, Mai C (2010) Effects of chemical modification of wood particles with glutaraldehyde and 1,3-dimethylol-4,5-dihydroxyethyleneurea on proper ties of the resulting polypropylene composites. Composit. Sci. Tech. 70: 2003-2011
Zhang Y, Bai Y, Yan B (2010) Functionalized carbon nanotubes for potential medicinal applications. Drug Disc. Today 15 (11): 428-435.
Received: 07/24/2015. Modified: 02/21/2019. Accepted: 02/23/2019.
Nelson Flores. Licenciado en Ingenieria Forestal, Instituto Tecnologico de Costa Rica. Consultor Privado. e-mail: firstname.lastname@example.org
Roger Moya (Autor de correspondencia). Bachiller en Ciencias Forestales, Universidade de Sao Paulo, Brasil, Investigador, Instituto Tecnologico de Costa Rica (ITCR). Direccion: Escuela de Ingenieria Forestal, ITCR. P.O. Box: 159-7050 Cartago-Costa Rica. e-mail: email@example.com
Ana Rodriguez-Zuniga. Doctora en Nanotecnologia, Universidad de Alicante, Espana. Profesora-Investigadora, ITCR, Costa Rica. e-mail: firstname.lastname@example.org
Jose Vega-Baudrit. Licenciado en Ingenieria Quimica, Universidad de Costa Rica. Consultor privado. email: email@example.com
Caption: Figure 1. Raman spectrum (532 nm excitation) (a) and thermographic analysis for MWCNT'sy MWCNT's-OH. Fuente: Moya et al. (2015a)
Caption: Figure 2. Average effort (MPa) modules of rupture (MOR) and modulus of elasticity (MOE) for nine tropical wood with two concentrations MWCNT's-OH (0.05% and 0.10%). Average values identified by the letters A and B are statistically different at [alpha]= 95%.
Caption: Figure 3. Mean axial and lateral hardness in nine tropical wood species with different concentrations MWCNT's-OH. Average values identified by the letters A and B are statistically different at [alpha] = 99%.
Caption: Figure 4. Shear stress parallel to the grain of nine tropical wood species with different concentrations MWCNT's-OH. Average values identified by the letters A and B are statistically different at [alpha] = 95%.
TABLE I RETENTION AND ABSORPTION OF NANOPARTICLES IN NINE TROPICAL SPECIES OF COSTA RICA FOR TWO CONCENTRATIONS OF MWCNT'S-OH Absorption of Retention of MWCNT's-OH MWCNT's-OH ([L.sub.solution]/ ([g.sub.nanotubes]/ [m.sup.3.sub.wood]) [m.sup.3.sub.wood] Species 0.05% 0.10% 0.05% 0.10% Acacia magnium 361 316 1.80 3.16 Cedrela odorata 218 214 1.08 2.14 Cordia alliodora 435 512 2.18 5.12 Enterolobium 307 328 1.54 3.28 cyclocarpum Gmelina arborea 283 257 1.42 2.57 Goethalsia meiantha 447 593 2.24 5.93 Ochroma pyramidale 380 266 1.90 2.67 Tectona grandis 271 311 1.36 3.11 Vochysia ferrugia 455 466 2.28 4.66 Wood density Species (kg/[m.sup.3]) Acacia magnium 533 Cedrela odorata 391 Cordia alliodora 346 Enterolobium 346 cyclocarpum Gmelina arborea 495 Goethalsia meiantha 399 Ochroma pyramidale 124 Tectona grandis 596 Vochysia ferrugia 544 TABLE II TENSION EFFORT IN NINE TROPICAL WOOD SPECIES WITH DIFFERENT CONCENTRATIONS MWCNT'S-OH Stress (MPa) Species 0% 0.05% 0.10% Acacia magnium 95.87 A 87.97 A 79.55 A Cedrela odorata 37.30 B 69.91 A 77.02 A Cordia alliodora 62.13 A 66.06 A 63.19 A Enterolobium cyclocarpum 30.59 A 31.51 A 35.84 A Gmelina arborea 66.56 A 65.59 A 61.49 A Goethalsia meiantha 57.07 B 75.79 A 61.99 B Ochroma pyramidale 30.75 A 26.32 A 31.01 A Tectona grandis 95.63 B 151.99 A 113.59 B Vochysia ferruginea 45.92 A 44.69 A 40.78 A Average values identified by the letters A and B are statistically different at [alpha] = 95%. TABLE III EFFORT IN COMPRESSION PARALLEL TO GRAIN IN NINE TROPICAL WOOD SPECIES WITH DIFFERENT CONCENTRATIONS OF MWCNT'S-OH Stress (MPa) Species 0% 0.05% 0.10% Acacia magnium 44.27 A 45.95 A 42.57 A Cedrela odorata 37.68 A 38.31 A 38.99 A Cordia alliodora 36.06 A 31.85 A 35.24 A Enterolobium cyclocarpum 29.41 A 33.58 A 33.70 A Gmelina arborea 37.21 B 48.75 A 40.69 B Goethalsia meiantha 35.89 AB 30.73 B 36.84 A Ochroma pyramidale 11.48 A 6.60 B 7.23 B Tectona grandis 40.83 A 42.11 A 41.55 A Vochysia ferrugia 28.89 A 25.81 A 27.59 A Note: Average values identified by the letters A and B are statistically different at [alpha] = 99%.
|Printer friendly Cite/link Email Feedback|
|Title Annotation:||texto en ingles|
|Author:||Flores, Nelson; Moya, Roger; Rodriguez-Zuniga, Ana; Vega-Baudrit, Jose|
|Date:||Feb 1, 2019|
|Previous Article:||VIDA DE ANAQUEL DE TILAPIA Oreochromis niloticus EVISCERADA TRANSPORTADA Y ALMACENADA EN HIELO.|
|Next Article:||VALOR SOCIOECONOMICO DE LAS PLANTAS PARA UNA COMUNIDAD INDIGENA TOTONACA.|